/ http://www.sciencemag.org/content/early/recent / 11 September 2014/ Page 1 / 10.1126/science.1254966
Downloaded from www.sciencemag.org on September 11, 2014
Detecting topological currents in graphene superlattices
1B). This approach, besides offering a direct probe of topological currents, provides a precision tool for mapping out the Berry curvature in G/hBN Bloch bands. We note that, so far, it has proven challenging to probe bulk topological currents without applying B. 1,2 3,4 1 2 R. V. Gorbachev, J. C. W. Song, G. L. Yu, A. V. Kretinin, F. This was the case, in particular, for the Withers,2 Y. Cao,1 A. Mishchenko,1 I. V. Grigorieva,2 K. S. anomalous Hall effect in magnetic metals, perhaps the cleanest system availaNovoselov,2 L. S. Levitov,3* A. K. Geim1,2* ble previously to study topological bulk 1 Centre for Mesoscience and Nanotechnology, University of Manchester, Manchester M13 9PL, UK. bands (6). 2 School of Physics and Astronomy, University of Manchester, Oxford Road, Manchester, M13 9PL, UK. Experimentally, we studied G/hBN 3 Department of Physics, Massachusetts Institute of Technology, Cambridge, MA 02139, USA. 4School of superlattices (in which the graphene Engineering and Applied Sciences, Harvard University, Cambridge, MA 02138, USA. and hBN lattices were aligned) fabri*Corresponding author. E-mail: [email protected]
(L.S.L.); [email protected]
(A.K.G.) cated following the procedures described in (21). Fifteen superlattice Topological materials may exhibit Hall-like currents flowing transversely to the devices similar to the one shown in the applied electric field even in the absence of a magnetic field. In graphene inset of Fig. 1B were investigated. The superlattices, which have broken inversion symmetry, topological currents charge carrier mobilities μ varied from originating from graphene’s two valleys are predicted to flow in opposite directions 40,000 to 80,000 cm2 V−1 s−1, and the and combine to produce long-range charge neutral flow. We observe this effect as a longitudinal and Hall resistivities (ρxx nonlocal voltage at zero magnetic field in a narrow energy range near Dirac points and ρxy, respectively) exhibited essenat distances as large as several microns away from the nominal current path. tially the same behavior as reported Locally, topological currents are comparable in strength to the applied current, previously (18, 19, 21, 22). Namely, indicating large valley-Hall angles. The long-range character of topological currents pronounced peaks in ρxx were observed and their transistor-like control by gate voltage can be exploited for information at the main neutrality point (NP) and at processing based on the valley degrees of freedom. carrier density n ≈ ±3 × 1012 cm−2 (Fig. 1B and fig. S1). The peaks in ρxx were accompanied by a sign reversal of ρxy Berry curvature is a physical field intrinsic to some crystal lattices, indicating the emergence of new NPs in the valence and conduction which can dramatically impact the transport properties of materials (1– bands of graphene (18–22). Both encapsulated and non-encapsulated 6). Topological effects, while known for some time (7), have gained structures were investigated, with the former having an additional hBN attention recently in connection with the discovery of topological insulacrystal placed on top of a G/hBN superlattice to protect it from environtors (8–11). In these materials, topological bands lead to new phenomena ment (20, 21). Some of the latter showed activation behavior at the main such as topologically protected edge-state transport in zero magnetic NP (fig. S2), yielding a bandgap 2∆ of 350 ± 40 K (20), in agreement field (12–14). No less striking, however, is the expected impact of Berry with the earlier transport (18, 19) and spectroscopy (23) measurements. curvature on bulk transport, leading to topological currents flowing perOur encapsulated devices, despite higher electronic quality, exhibited no pendicular to the applied electric field E (5, 6). The nondissipative nature activation behavior at the main NP, with the ρxx value saturating at 100 Ohm) over the entire range of acces-
sible n (Figs. 1 and 2 and fig. S1), RNL decays rapidly with n and completely disappears under noise for densities >1011 cm−2 away from the α NPs. The dependence can be approximately described by RNL ∝ 1 n with α ≈ 2.5-3 (Fig. 2B). A nonlocal voltage can also appear due to stray charge currents, described by the van der Pauw relation (24) RNL ~ ρxx exp(–πL/w) where L is the distance between the current path and voltage probes and w the device width (Fig. 1B, micrograph). For typical aspect ratios L/w ≈ 4, the formula yields ≈0.01 Ohm. The magnitude of this contribution and its n dependence, which follows ρxx(n), are clearly incompatible with the observed nonlocal response. We have also investigated how RNL depends on L and found an exponential dependence exp(–L/ξ) with ξ ≈1.0 μm (Fig. 2C). This ξ value is close to w and much larger than the elastic mean free path of ≈0.1 μm estimated from μ for the range of n where RNL appears. Furthermore, RNL exponentially decreases with increasing T so that no nonlocal signal is detected above 150 K whereas ρxx remains large at this T at the main NP (figs. S2 and S3). Non-encapsulated devices exhibited practically the same behavior of RNL as a function of n and T (fig. S4) but the absolute value of RNL was somewhat smaller than that in encapsulated devices (20). In addition, we investigated the effect of charge inhomogeneity δn on RNL, which was controlled by sweeping to progressively larger gate voltages Vg beyond the hole-side NP (20). When δn was increased by a factor of ≈2, RNL could sometimes change by more than an order of magnitude (20). The inhomogeneity enhanced RNL at the main NP and suppressed it at the hole-side NP (fig. S5). The difference is attributed to a narrow energy width of the secondary Dirac spectrum (20). To confirm the key role played by Berry curvature, we verified that the nonlocal response was absent in G/hBN systems without alignment and, accordingly, with no detectable superlattice effects (18–22). This is illustrated in Fig. 2A that shows RNL for aligned and nonaligned devices with the same μ and in the same geometry. In the nonaligned devices (>20 measured), no nonlocal signal could be observed even at our maximum resolution of ∼0.1 ohm (Fig. 2A, blue curve). Therefore, the observed RNL cannot be explained by charge-neutral flow of spin and/or energy, which are indifferent to crystal alignment. The latter flows also require broken TRS and completely disappear in zero B as reported previously (24–26). In our superlattice devices, a contribution of spin/energy flows becomes appreciable only for B > 0.1 T (fig. S6), leading to rapid broadening of the RNL peaks, in agreement with ref. 24. We have also considered the possibility that the observed nonlocality at B=0 may originate from an edge transport mechanism. For example, topological materials can support gapless edge modes that coexist with the gapped bulk. Such modes could in principle mediate nonlocal charge transport. However, our experiments provide no evidence for metallic conductivity along the device edges. First, the measured nonlocal response was similar for all our devices, independent of whether they exhibited metallic or insulating behavior in ρxx. Second, AFM studies show that the moiré pattern associated with the alignment extends all the way to the device edges and there are no distinct edge regions (19). Third, extrapolating the dependence in Fig. 2C to small L, we find that the edge transport scenario would require metallic conductivity along edges of ≈2e2/h over distances of L > 1 μm. This would imply perfect edge state transport, which is unlikely at such length scales in the presence of strong intervalley scattering expected at microscopically rough edges. Proceeding with the analysis, we note that the aligned superlattices are comprised of hexagonal unit cells, each representing a commensurate graphene/hBN region of ∼10 nm in size, which is surrounded by a strained boundary (19). All unit cells are characterized by A/B sublattice asymmetry of the same sign, giving a preferred chirality over the entire structure (19, 20, 25). For our typical n < 1011 cm−2, Fermi wavelengths are larger than 100 nm, which exceeds the superlattice periodicity by a factor of ∼10. This large wavelength/period ratio renders contributions from spatially varying couplings insignificant.
We will show below that the observed nonlocality features are consistent with bulk topological currents expected for a gapped Dirac spectrum. The mechanism by which Berry curvature generates topological currents can be elucidated by the semiclassical equations of motion (5) 1 ∂ ( k ) , v(k ) + k × Ω ( k ) (1) k = eE + ev ( k ) × B= ∂k where Ω is the Berry curvature density and v(k) the group velocity of Bloch electrons. The Lorentz force term ev × B describes the conventional Hall effect. Berry curvature gives rise to an ‘anomalous velocity’, k × Ω ( k ) , which is of the same structure as the Lorentz term but in momentum space and leads to transverse currents (Fig. 1A). Such currents may appear in zero B [without breaking TRS that requires Ω(k) = −Ω(−k)] as long as inversion symmetry is broken, Ω(k) ≠ Ω(−k), as is the case of our aligned devices with the globally broken sublattice A/B symmetry (19). For B = 0, transverse currents arise solely from Ω(k), yielding Hall-like conductivity σxy given by the sum of Berry fluxes for all occupied states in the Fermi sea (3) e2 d 2k = σ xy 2 ∫ Ω ( k ) f ( k ) (2) h 2π with f(k) being the Fermi function and the factor of 2 accounting for spin degeneracy. Because Berry curvature is odd in energy (20), σxy has the same sign for both electrons and holes. This contrasts with the conventional Hall conductivity that is sign-changing under carrier-type reversal. As a result, σxy given by Eq. 2 is less susceptible to smearing by inhomogeneity. This mechanism yields a nonzero RNL whenever the Fermi level is tuned through Berry curvature hot spots. Their extent in energy is given by half the bandgap Δ ≈ 180 K, which translates into n ≈ 2 × 1010 cm−2 and agrees well with the ultra-narrow width of our RNL peaks. Because of TRS, the electric field generates topological currents (Eq. 1) with opposite transverse components in graphene’s two valleys, K and K′ (Fig. 1A), to create the charge-neutral VHE, J v =− JK JK′ = σvxy E , v where σ xy = 2σ xy . As illustrated in the inset to Fig. 1B, topological currents can result in a VHE conductivity of ≈2e2/h. In the absence of intervalley scattering, the charge-neutral currents can persist over extended distances and mediate nonlocal electrical signals (24–28). The resulting nonlocal resistance RNL can be understood as originating from the VHE and a reverse VHE (20), by analogy with nonlocal transport mediated by charge-neutral spin or energy flow (24–28). Yet, unlike the latter, the VHE-induced nonlocality appears without TRS breaking, that is, at zero B. This behavior, as well as the narrow range of n over which RNL is observed, is a telltale sign of bulk topological currents. The analysis outlined above yields the model expression (20)
( w 2ξ ) ( σvxy )
ρ3xx exp ( − L ξ ) (3).
The peak in RNL(n) can be described by Eq. 3 with no fitting parameters (Fig. 2B). The measured spatial decay with ξ ≈ 1.0 μm is consistent with intervalley scattering occurring at graphene edges and/or at atomic-scale defects (20). The large values of RNL at L of several μm also imply extremely strong topological currents locally, within the path of the applied current. By extrapolating the observed L dependence to L